LMucko/crystallography-open-database huggingface dataset:
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 900 deg C for 2 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002738
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 900 deg C for 2 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0836
_cell_length_b                   8.0836
_cell_length_c                   8.0836
_cell_volume                     528.220
_database_code_amcsd             0002827
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 900 deg C for 2 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002738
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 900 deg C for 5 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002739
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 900 deg C for 5 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0838
_cell_length_b                   8.0838
_cell_length_c                   8.0838
_cell_volume                     528.259
_database_code_amcsd             0002828
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 900 deg C for 5 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002739
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 900 deg C for 60 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002740
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 900 deg C for 60 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al1.999 Mg1.001 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0837
_cell_length_b                   8.0837
_cell_length_c                   8.0837
_cell_volume                     528.239
_database_code_amcsd             0002829
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 900 deg C for 60 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg1.001 Al1.999) O4'
_cod_database_code               9002740
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 900 deg C for 4320 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002741
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 900 deg C for 4320 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0838
_cell_length_b                   8.0838
_cell_length_c                   8.0838
_cell_volume                     528.259
_database_code_amcsd             0002830
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
;annealed at 1000 deg C for 12h; isothermally ordered at 900 deg C for 4320
 min
;
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002741
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002742
_publ_section_title
;
 Kinetics of cation ordering in synthetic MgAl2O4 spinel
 Sample: annealed at 1000 deg C for 12h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0835
_cell_length_b                   8.0835
_cell_length_c                   8.0835
_cell_volume                     528.200
_database_code_amcsd             0002831
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history   'annealed at 1000 deg C for 12h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002742
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 2 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002743
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 2 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al1.999 Mg1.001 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0834
_cell_length_b                   8.0834
_cell_length_c                   8.0834
_cell_volume                     528.180
_database_code_amcsd             0002832
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 2 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg1.001 Al1.999) O4'
_cod_database_code               9002743
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 5 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002744
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 5 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0836
_cell_length_b                   8.0836
_cell_length_c                   8.0836
_cell_volume                     528.220
_database_code_amcsd             0002833
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 5 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002744
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 10 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002745
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 10 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0840
_cell_length_b                   8.0840
_cell_length_c                   8.0840
_cell_volume                     528.298
_database_code_amcsd             0002834
_exptl_crystal_density_diffrn    3.577
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 10 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002745
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 20 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002746
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 20 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2.001 Mg0.999 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0843
_cell_length_b                   8.0843
_cell_length_c                   8.0843
_cell_volume                     528.357
_database_code_amcsd             0002835
_exptl_crystal_density_diffrn    3.577
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 20 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg.999 Al2.001) O4'
_cod_database_code               9002746
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 40 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002747
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 40 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2.001 Mg0.999 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0844
_cell_length_b                   8.0844
_cell_length_c                   8.0844
_cell_volume                     528.376
_database_code_amcsd             0002836
_exptl_crystal_density_diffrn    3.577
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 40 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg.999 Al2.001) O4'
_cod_database_code               9002747
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 150 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002748
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 150 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0846
_cell_length_b                   8.0846
_cell_length_c                   8.0846
_cell_volume                     528.416
_database_code_amcsd             0002837
_exptl_crystal_density_diffrn    3.577
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 150 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002748
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 1440 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002749
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 1440 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al1.999 Mg1.001 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0845
_cell_length_b                   8.0845
_cell_length_c                   8.0845
_cell_volume                     528.396
_database_code_amcsd             0002838
_exptl_crystal_density_diffrn    3.577
_exptl_crystal_thermal_history
;annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 1440
 min
;
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg1.001 Al1.999) O4'
_cod_database_code               9002749
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 800 deg C for 10080 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002750
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 800 deg C for 10080 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0846
_cell_length_b                   8.0846
_cell_length_c                   8.0846
_cell_volume                     528.416
_database_code_amcsd             0002839
_exptl_crystal_density_diffrn    3.577
_exptl_crystal_thermal_history
;annealed at 1000 deg C for 12h; isothermally ordered at 800 deg C for 10080
 min
;
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002750
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h
Andreozzi G B; Princivalle F; American Mineralogist 87 (2002) 838–844; doi:

data_9002751
_publ_section_title
;
 Kinetics of cation ordering in synthetic MgAl2O4 spinel
 Sample: annealed at 1000 deg C for 12h
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al2 Mg O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0832
_cell_length_b                   8.0832
_cell_length_c                   8.0832
_cell_volume                     528.141
_exptl_crystal_thermal_history   'annealed at 1000 deg C for 12h'
_cod_duplicate_entry             9002734
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al2) O4'
_cod_database_code               9002751
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 700 deg C for 10 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002752
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 700 deg C for 10 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al1.999 Mg1.001 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0831
_cell_length_b                   8.0831
_cell_length_c                   8.0831
_cell_volume                     528.122
_database_code_amcsd             0002841
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 700 deg C for 10 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg1.001 Al1.999) O4'
_cod_database_code               9002752
Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at 1000 deg C for 12h, then isothermally ordered at 700 deg C for 60 min
Andreozzi, G. B.; Princivalle, F.; American Mineralogist 87 (2002) 838–844; doi:

data_9002753
_publ_section_title
;Kinetics of cation ordering in synthetic MgAl2O4 spinel Sample: annealed at
 1000 deg C for 12h, then isothermally ordered at 700 deg C for 60 min
;
_journal_name_full               'American Mineralogist'
_journal_page_first              838
_journal_page_last               844
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Al1.999 Mg1.001 O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0838
_cell_length_b                   8.0838
_cell_length_c                   8.0838
_cell_volume                     528.259
_database_code_amcsd             0002842
_exptl_crystal_density_diffrn    3.578
_exptl_crystal_thermal_history
'annealed at 1000 deg C for 12h; isothermally ordered at 700 deg C for 60 min'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg1.001 Al1.999) O4'
_cod_database_code               9002753